Baixe grátis o arquivo ASTM Apdf enviado por DANIEL no curso de Engenharia Mecânica. Sobre: Astm a ASTM A/AM(98), Austenitic, corrosion resistant, solution quenched and aged. 21 Sep Articles. Microstructure and Mechanical Properties of ASTM A CA6NM Steel Welded by.
|Published (Last):||19 May 2010|
|PDF File Size:||10.66 Mb|
|ePub File Size:||2.38 Mb|
|Price:||Free* [*Free Regsitration Required]|
ASTM A743 CF3M, 316L stainless steel casting
Figure 4 illustrates the location of the microhardness measurements, including the base metal, weld metal and heat-affected zone. Low toughness reduces the life of the piece and accelerates the process of cavitation as well 7.
Incrivelmente absorvente do primeiro ao However, the PWHT material has shown finely dispersed retained austenite, in an amount near 10 vol. In addition, as mentioned before, no detectable defect has been found through X-ray analysis. The Charpy V-Notch results of HAZ zone of both materials are higher than those of the weld metal, reaching values as high as J, likely associated to the presence of some tough base metal in the crack propagation path.
How to cite this article. The weld joints were free of defects such as cracks, porosity, a43 entrapment, lack of fusion and incomplete penetration. Or if you don’t have an account with us yet, then click here to register.
We advise that you only use the original value or one of its raw conversions in your calculations to minimize rounding error.
American Society of Mechanical Engineers; This abstract is a brief summary of the referenced standard. Please contact us at webmaster matweb.
The microstructure and mechanical properties of the as-welded joint was compared to a joint which suffered a post welding heat treatment PWHT. X-ray diffraction was used to check the phases present, mainly retained austenite. Welding Metallurgy of Stainless Steels.
CF16a | A Stainless Steel | MetalTek
It should be pointed out that this retained austenite is hardly observed by conventional metallographic techniques 6. For analysis by optical microscopy, the samples were submitted to usual metallographic preparation procedures involving cutting; grinding, polishing and etching with Vilella reagent that consists in 5 g if picric acid, 2.
In the present work, more Charpy coupons where tested as satm The authors would like to express their gratitude to Dr. It is the most common metallic alloy used in the manufacture of this type zstm equipment, replacing -Mn steels by offering better resistance against corrosion and cavitation damage 2.
CA6NM sstm is widely used in the manufacture of hydraulic turbines metallic parts, due to its resistance to corrosion and cavitation damage, combined with good weldability and fatigue properties. Effect of delta ferrite on impact properties of low carbon 13Cr-4Ni martensitic stainless steel. Historical Version s – view previous versions of standard.
There are pictures of 50x magnification creating a mosaic, for better visualization of the weld joints and their integrity. The low-carbon Martensitic steels CA6NM is offset with the addition of nickel, whose purpose is to expand the austenitic field, Therefore, keep the potential and enable complete austenitization and also to temper with the formation of martensite.
ABSTRACT CA6NM steel is widely used in the manufacture of hydraulic turbines metallic ast, due to its resistance to corrosion and cavitation damage, combined with good weldability and fatigue properties. Regions R and C present a more refined microstructure compared to the upper asstm Tlikely associated to a larger number of heat cycles suffered by these regions as consequence of the greater number of weld passes over these regions.
Originally approved in Results and Discussions Figure 5 illustrates mosaics of the weld joints obtained by using a motorized optical microscope OM. Failure to comply with the general requirements of Specification A constitutes nonconformance with this specification.
The castings shall be subjected to heat treatment.
Cast Grade: CF16a
Effect of d-ferrite on impact properties of supermartensitic stainless steel heat affected zones. Data sheets for overmetals, plastics, ceramics, and composites. Current edition approved March ashm, The two joints were X-ray tested and have not presented any detectable defects. In addition, a smoother hardness values distribution is observed among the different regions of the PWHT sample, making the hardness values of the weld metal close to those of base metal.